Synthesis of SDS-Modified Pt/Ti3C2Tx Nanocomposite Catalysts and Electrochemical Performance for Ethanol Oxidation

It is well-known that platinum (Pt) is still the preferred material of anode catalyst in ethanol oxidation, however, the prohibitive high cost and CO poisoning of Pt metal impede the commercialization of fuel cells. Therefore, improving the utilization rate of catalysts and reduce the cost of catalyst become one of the most concerned focus in the construction of fuel cells. In this work, the Pt-based catalysts are synthesized by using different content of sodium dodecyl sulfate (SDS) modified-Ti3C2Tx support, and the dispersion regulation function of SDS modified-Ti3C2Tx supported on Pt nanoparticles is investigated. The structure, composition and morphology of different catalysts are characterized by X-ray diffraction (XRD), X-ray spectroscopy (EDX), transmission electron microscopy (TEM) and high-resolution TEM, respectively. It is found that the Pt nanoparticles in pure Ti3C2Tx surface are serious aggregated and show poor dispersion, whereas the Pt nanoparticles in SDS modified-Ti3C2Tx have a better dispersion. The electrochemical results revealed that SDS modified-Ti3C2Tx supported Pt nanoparticles has higher electrocatalytic activity and stability in both acidic and alkaline ethanol oxidation when the dosage of SDS increases to 100 mg. These findings indicate that the SDS-Ti3C2Tx/Pt catalysts show a promising future of potential applications in fuel cells with modification of Ti3C2Tx support.


Introduction
With the continuous energy consumption and population growth, energy crisis has been a big problem of the world. In recent years, metal-air batteries (Li, Na, Zn) exhibit higher theoretical specific energy than traditional lithium ion batterie [1,2], however stateof-art metal-air batteries still produce performance that are well below practical levels. In contrast to the metal-air batteries, liquid fuel cell can be considered as a decent compromise between LIBs and metal-air batteries. Direct ethanol fuel cell (DEFC) is a liquid fuel cell with the advantages of high energy density, low environmental pollution, simple equipment structure, and easy preparation [3][4][5][6][7][8][9]. Platinum-based materials are generally used as the anode catalyst towards ethanol oxidation due to their excellent electrocatalytic performance. With the development of nanotechnology, researchers tend to design and synthesize nano-catalysts with controllable size and morphology, which could improve their catalytic activity. Liang et al. improved the stability of platinum-based catalysts by doping other atoms [10]. However, pure platinum catalyst is still expensive and can be easily poisoned by the intermediates from alcohol oxidation, limiting its commercial application in DEFC [11][12][13][14][15]. To resolve this problem, a more effective way is to explore a suitable catalyst carrier where the Pt nanoparticles can be uniformly dispersed and be well stabilized for a high catalytic efficiency.

Synthesis of Ti 3 C 2 T x
Ti 3 C 2 T x was prepared by etching method in the HCl+LiF mixed solution. Firstly, 1.6 g LiF was added to 20 mL 9 mol L −1 HCl, stir at 35 • C for half an hour, so that LiF was completely dissolved in HCl to obtain a transparent etching solution, and then Ti 3 AlC 2 was slowly added to the HCl+LiF etching solution under stirring. In order to avoid violent exothermic reaction, stirring was kept for 24 h. The precipitated product was washed with ethanol and deionized water until the pH value of the supernatant was close to neutral. Finally, the product was placed in a vacuum oven to dry for 12 h, and the resultant was Ti 3 C 2 T x powder.

Preparation of Ti 3 C 2 T x -Pt Composites Modified with Different Content of SDS
First, 1.0 g H 2 PtCl 6 was dissolved in 250 mL of distilled water to form a solution with a concentration of 7.723 mmol L −1 . 40 mg Ti 3 C 2 T x powder prepared in the previous step was added to 40 mL deionized water, and ultrasonicated for 2 h. The SDS was employed as the surfactant to prevent the produced Pt nanoparticles to aggregation. In order to study the effect of SDS amounts on the electrocatalytic performance, different contents of SDS were added into the Ti 3 C 2 T x solution and ultrasonicated for another 30 min. We set up four sets of samples, where 0 mg, 20 mg, 50 mg, and 100 mg of SDS were added into the Ti 3 C 2 T x solution and the subsequent operations were the same as above. After then, 6.5 mL H 2 PtCl 6 (7.723 M) solution was added the above solution under a magnetic stirrer for rapid stirring. 60 mg of NaBH 4 solid was dissolved in 10 mL of deionized water, and the resulting solution was added to the above-mentioned H 2 PtCl 6 -Ti 3 C 2 T x solution, and stirring was continued for 4 h. Then, the product was obtained by centrifugation, and washed twice with deionized water and ethanol successively. Finally, the product was put into an oven to dry at 60 • C for 12 h.

Characterization
X-ray powder diffractometer (XRD), scanning electron microscopy (SEM) and transmission electron microscopy (TEM) were applied to characterize and analyze the morphology and structure of the prepared samples. The samples were carried on Fourier transform infrared spectroscopy (FTIR) with a Nicolet 6700 FTIR spectrometer instrument using a KBr pellet, and Raman spectrometer (LABRAM-1B) with a 514 nm laser source. The oxidation states of and samples were obtained by X-ray photoelectron spectroscopy (XPS, XSAM800 Ultra spectrometer). A three-electrode system was used to conduct electrochemical tests by the CHI660E electrochemical workstation. The reference electrode was a saturated calomel electrode, the counter electrode was a platinum electrode, and the working electrode was a glassy carbon electrode coated with the prepared catalysts (working area is 0.07 cm 2 ).The working electrode was prepared as follows: 5 mg of catalyst powder was dissolved in a mixed solution consisting of 850 µL of deionized water, 100 µL of isopropanol and 50 µL of Nafion, and then ultrasonicated for half an hour to form a uniformly dispersed catalyst solution. 10 µL of the catalyst solution was hanging dropped on the surface of the polished glassy carbon electrode by pipette and dried under infrared lamp. The commercial JM 20 wt% Pt/C catalyst was prepared by the same procedure.

Physical Characterization
The preparation process of the SDS-modified Ti 3 C 2 T x -Pt composite material was shown in Figure 1. First, the Ti 3 AlC 2 powder was etched into a multilayer structure by LiF and HCl. Then, the multilayer Ti 3 C 2 T x is modified with SDS and sonicated into SDSmodified Ti 3 C 2 T x support, and the Pt nanoparticles is deposited on the SDS-modified Ti 3 C 2 T x support by serving NaBH 4 as reducing expanded graphite after the Al layer was selectively removed under etching. It can be found from the SEM (Figure 2a) that the obtained Ti 3 C 2 T x exhibits an accordion layered structure, the TEM (Figure 2b) image and EDX mapping show a thin and semitransparent nanosheet with a uniform distribution of the Ti and C elements from Ti 3 C 2 T x . The structure of as-prepared SDS-Ti 3 C 2 T x /Pt composites were analyzed by X-ray powder analyzer and the results were shown in Figure 3. In Figure 3a, a series of strong and sharp characteristic diffraction peaks are observed in the initial T i3 AlC 2 powder, corresponding to the hexagonal crystal (JCPDS. No.520875). After etching, original characteristic peaks disappear, and new peaks associated with Ti 3 C 2 T x were appears, indicating the successful synthesis of Ti 3 C 2 T x . Figure 3b shows the XRD spectra of the 0-SDS-Ti 3 C 2 T x /Pt, 20-SDS-Ti 3 C 2 T x /Pt, 50-SDS-Ti 3 C 2 T x /Pt, and 100-SDS-Ti 3 C 2 T x /Pt. Most of the nanocomposites show the Ti 3 C 2 T x characteristic diffraction peaks at 2θ = 33.9 • , 38.  [26,27]. In addition, SDS-modified Ti 3 C 2 T x -Pt composite nearly resembles the pure Ti 3 C 2 T x in terms of the position of Raman bands, only the vibration mode at 482 cm −2 is gradually disappeared when the SDS increased to 50 mg ( Figure S1). The result revealed the A 1g out-of-plane vibration modes at 154 and 619 cm −2 for C and Ti atoms, and the E g in-plane vibration modes at 207 and 333 cm −2 for C, Ti and surficial groups [28]. FT-IR spectra ( Figure S2) manifests the rich surface chemistry of MXene structure by the adsorption peaks corresponding to -OH asymmetric stretch (3446 cm −1 ), -OH asymmetric vibration (2916 cm −1 ), -OH bending vibration (1627 cm −1 ), Ti-C-O (1107 cm −1 ), which is consisted with the previous work [29]. and HCl. Then, the multilayer Ti3C2Tx is modified with SDS and sonicated into SDS--modified Ti3C2Tx support, and the Pt nanoparticles is deposited on the SDS--modified Ti3C2Tx support by serving NaBH4 as reducing expanded graphite after the Al layer was selectively removed under etching. It can be found from the SEM (Figure 2a) that the obtained Ti3C2Tx exhibits an accordion layered structure, the TEM (Figure 2b) image and EDX mapping show a thin and semitransparent nanosheet with a uniform distribution of the Ti and C elements from Ti3C2Tx. The structure of as-prepared SDS-Ti3C2Tx/Pt composites were analyzed by X-ray powder analyzer and the results were shown in Figure 3. In Figure 3a, a series of strong and sharp characteristic diffraction peaks are observed in the initial Ti3AlC2 powder, corresponding to the hexagonal crystal (JCPDS. No.520875). After etching, original characteristic peaks disappear, and new peaks associated with Ti3C2Tx were appears, indicating the successful synthesis of Ti3C2Tx. Figure [26,27]. In addition, SDS-modified Ti3C2Tx-Pt composite nearly resembles the pure Ti3C2Tx in terms of the position of Raman bands, only the vibration mode at 482 cm −2 is gradually disappeared when the SDS increased to 50 mg ( Figure S1). The result revealed the A1g out-of-plane vibration modes at 154 and 619 cm −2 for C and Ti atoms, and the Eg in-plane vibration modes at 207 and 333 cm −2 for C, Ti and surficial groups [28]. FT-IR spectra ( Figure S2) manifests the rich surface chemistry of MXene structure by the adsorption peaks corresponding to -OH asymmetric stretch (3446 cm −1 ), -OH asymmetric vibration (2916 cm −1 ), -OH bending vibration (1627 cm −1 ), Ti-C-O (1107 cm −1 ), which is consisted with the previous work [29].     XPS measurements were further used to analyze the composition and surface oxidation state of the as-prepared catalysts. Figure 4 shows the high-resolution XPS spectra of 0-SDS-Ti3C2Tx/Pt, 20-SDS-Ti3C2Tx/Pt, 50-SDS-Ti3C2Tx/Pt and 100-SDS-Ti3C2Tx/Pt catalysts. As observed, the survey spectra evidenced the existence of C, Ti, Pt, O elements and the similar position for the four catalysts. As shown in Figure 4a, the SDS-Ti3C2Tx/Pt displays two prominent peaks at binding energies of 70.7 and 73.9 eV, corresponding to the Pt 4f7/2 and Pt 4f5/2 of metallic Pt [30]. The Ti 2p spectrum could be deconvoluted into two peaks at 464.1 and 458.3 eV, which can be ascribed to the Ti-O (2p1/2) and Ti-O (2p3/2) group, respectively ( Figure 4b). For the XPS spectra of C 1s, the two peaks at 284.4 and 285.5 eV seen in Figure 4c correspond to the C-C and O=C-OH group, respectively. The peaks with binding energies of 529.9, 531.4 and 532.3 eV can be assigned to the Ti-O, chemisorbed or physically absorbed oxygen and Ti-OH species (Figure 4d), indicating the presence of abundant surface oxygenated groups on the surface of Ti3C2Tx [20]. In order to determine the effect of the surfactant SDS content on the morphology and dispersibility of Pt nanoparticles, the microstructure of the nanocomposite catalyst was observed in Figure 5. It can be seen from Figure 5a that Pt nanoparticles are severely agglomerated on the Ti3C2Tx carrier without SDS modification. However, when the Ti3C2Tx is modified by SDS, Pt na- XPS measurements were further used to analyze the composition and surface oxidation state of the as-prepared catalysts. Figure 4 shows the high-resolution XPS spectra of 0-SDS-Ti 3 C 2 T x /Pt, 20-SDS-Ti 3 C 2 T x /Pt, 50-SDS-Ti 3 C 2 T x /Pt and 100-SDS-Ti 3 C 2 T x /Pt catalysts. As observed, the survey spectra evidenced the existence of C, Ti, Pt, O elements and the similar position for the four catalysts. As shown in Figure 4a, the SDS-Ti 3 C 2 T x /Pt displays two prominent peaks at binding energies of 70.7 and 73.9 eV, corresponding to the Pt 4f 7/2 and Pt 4f 5/2 of metallic Pt [30]. The Ti 2p spectrum could be deconvoluted into two peaks at 464.1 and 458.3 eV, which can be ascribed to the Ti-O (2p 1/2 ) and Ti-O (2p 3/2 ) group, respectively ( Figure 4b). For the XPS spectra of C 1s, the two peaks at 284.4 and 285.5 eV seen in Figure 4c correspond to the C-C and O=C-OH group, respectively. The peaks with binding energies of 529.9, 531.4 and 532.3 eV can be assigned to the Ti-O, chemisorbed or physically absorbed oxygen and Ti-OH species (Figure 4d), indicating the presence of abundant surface oxygenated groups on the surface of Ti 3 C 2 T x [20]. In order to determine the effect of the surfactant SDS content on the morphology and dispersibility of Pt nanoparticles, the microstructure of the nanocomposite catalyst was observed in Figure 5. It can be seen from Figure 5a that Pt nanoparticles are severely agglomerated on the Ti 3 C 2 T x carrier without SDS modification. However, when the Ti 3 C 2 T x is modified by SDS, Pt nanoparticles are uniformly dispersed and exhibit a smaller particle size on the Ti 3 C 2 T x surface, as shown in Figure 5b-d. In addition, the more content of the SDS surfactant is added, the better dispersion of Pt nanoparticles could be achieved. Generally speaking, nanoparticles with a smaller particle size and better dispersion provide more active sites for electrochemical reactions, thereby increasing the catalytic activity [31]. noparticles are uniformly dispersed and exhibit a smaller particle size on the Ti3C2Tx surface, as shown in Figure 5b-d. In addition, the more content of the SDS surfactant is added, the better dispersion of Pt nanoparticles could be achieved. Generally speaking, nanoparticles with a smaller particle size and better dispersion provide more active sites for electrochemical reactions, thereby increasing the catalytic activity [31].      Figure 6b, the interplanar spacing of 0.251 nm is observed, which is consistent with the Pt (200) crystal-plane in Figure 6a. In addition, the EDX spectrum in Figure 6c also confirms the presence of Pt in the nanocomposite catalyst. Among them, the peaks of C and Ti are mainly derived from Ti 3 C 2 T x , and the signal of the O peak is attributed to the oxygen-containing functional groups of Ti 3 C 2 T x and the surface oxygen of copper mesh. Figure 6d shows the EDX mapping, in which a uniform distribution of the Ti, C and O elements from Ti 3 C 2 T x nanosheets is observed, while the Pt element is highly dispersed on the Ti 3 C 2 T x nanosheets in the form of small Pt nanoparticles.   Figure 6b, the interplanar spacing of 0.251 nm is observed, which is consistent with the Pt (200) crystal-plane in Figure 6a. In addition, the EDX spectrum in Figure 6c also confirms the presence of Pt in the nanocomposite catalyst. Among them, the peaks of C and Ti are mainly derived from Ti3C2Tx, and the signal of the O peak is attributed to the oxygen-containing functional groups of Ti3C2Tx and the surface oxygen of copper mesh. Figure 6d shows the EDX mapping, in which a uniform distribution of the Ti, C and O elements from Ti3C2Tx nanosheets is observed, while the Pt element is highly dispersed on the Ti3C2Tx nanosheets in the form of small Pt nanoparticles.

Electrochemical Characterization
In order to study the electrocatalytic activity of the catalyst, cyclic voltammetry (CV) curves were used to investigate the electrocatalytic activity of different catalysts in the acidic ethanol and the alkaline ethanol. The CV curves of 0-SDS-Ti3C2Tx/Pt, 20-SDS-Ti3C2Tx/Pt, 50-SDS-Ti3C2Tx/Pt and 100-SDS-Ti3C2Tx/Pt catalysts in 0.5 mol L −1 H2SO4 solution were measured. As shown in Figure 7a, the cathode and anode peaks with the potential range of −0.2 V to 0.1 V correspond to the absorption peak and desorption peak of

Electrochemical Characterization
In order to study the electrocatalytic activity of the catalyst, cyclic voltammetry (CV) curves were used to investigate the electrocatalytic activity of different catalysts in the acidic ethanol and the alkaline ethanol. The CV curves of 0-SDS-Ti 3 C 2 T x /Pt, 20-SDS-Ti 3 C 2 T x /Pt, 50-SDS-Ti 3 C 2 T x /Pt and 100-SDS-Ti 3 C 2 T x /Pt catalysts in 0.5 mol L −1 H 2 SO 4 solution were measured. As shown in Figure 7a, the cathode and anode peaks with the potential range of −0.2 V to 0.1 V correspond to the absorption peak and desorption peak of monolayer hydrogen under acidic conditions, respectively. The electrochemically active area (ECSA) of the electrode can be estimated from the peak area of the hydrogen absorption and desorption [32,33]. ECSA = Q h /(0.21 × m), where Q h represents the amount of electricity during hydrogen desorption, and m is the content of Pt on the electrode. According to this formula, the ECSA of 100-SDS-Ti 3 C 2 T x /Pt, 50-SDS-Ti 3 C 2 T x /Pt, 20-SDS-Ti 3 C 2 T x /Pt, 0-SDS-Ti 3 C 2 T x /Pt nanocomposite catalyst is 9.02, 5.67, 2.60, 1.80 m 2 g −1 , respectively. The larger ECSA is, the higher catalytic activity is achieved in the acidic media. Figure 7b shows the CV curve of 0-SDS-Ti 3 C 2 T x /Pt, 20-SDS-Ti 3 C 2 T x /Pt, 50-SDS-Ti 3 C 2 T x /Pt, and 100-SDS-Ti 3 C 2 T x /Pt nanocomposites in 1 mol L −1 KOH solution. The sweep potential range is −1.0 V~0.2 V. As shown in this figure, during the reverse scanning process, all catalysts have obvious redox peaks at −0.25 V. Among these catalysts, the 100-SDS-Ti 3 C 2 Tx /Pt catalyst has the largest peak current density, indicating the highest electrocatalytic activity. As mentioned above, the ECSA value of 100-SDS-Ti 3 C 2 T x /Pt is obvious higher that of 50-SDS-Ti 3 C 2 T x /Pt, 20-SDS-Ti 3 C 2 T x /Pt and 0-SDS-Ti 3 C 2 T x /Pt electrode, rendering the highest electrochemical activity among these catalysts. This is attributed to the better dispersion of catalyst nanoparticles on the surface of Ti 3 C 2 T x with more SDS surfactant, which increases the more active sites for electrochemical reactions. electrochemical activity among these catalysts. This is attributed to the better dispersion of catalyst nanoparticles on the surface of Ti3C2Tx with more SDS surfactant, which increases the more active sites for electrochemical reactions.  Figure 8a shows the CV curves of the four nanocatalysts in 0.5 mol L −1 H2SO4+1 mol L −1 C2H5OH solution. There are two obvious oxidation peaks observed at 0.65 V and 0.46 V, which is assigned to the positive oxidation peak of ethanol and the oxidation peak of the toxic intermediate product during the negative scan. Generally, a higher the peak current of ethanol during forward scanning means a better catalytic performance. The current density of the 100-SDS-Ti3C2Tx/Pt nanocatalyst reaches 50.3 mA cm −2 , which is much higher than 0-SDS-Ti3C2Tx/Pt, 20-SDS-Ti3C2Tx/Pt, and 50-SDS-Ti3C2Tx/Pt, indicating its largest electrocatalytic activity. The ratio (jf/jb) between the current density of the positivescan oxidation peak (jf) and the peak current density (jb) of the anti-scan oxidation peak (jf/jb) is employed to study the anti-toxicity of the catalyst during the ethanol oxidation process. The higher ratio (jf/jb) is, the easier oxidation reaction of ethanol is, and the nanocomposite can adsorb ethanol molecules more efficiently [34,35]. As shown in Figure 8b, it can be clearly found the jf/jb value of 100-SDS-Ti3C2Tx/Pt catalyst is 1.21, which is higher than 50-SDS-Ti3C2Tx/Pt (1.17), 20-SDS-Ti3C2Tx/Pt (0.94), and 0-SDS-Ti3C2Tx/Pt (0.97), further demonstrating its high electrocatalytic activity and anti-poisoning ability for ethanol oxidation in acidic media. Owing to the superior electrocatalytic activity of 100-SDS-Ti3C2Tx/Pt over other catalyst, we also compared the electrochemical performance of 100-SDS-Ti3C2Tx/Pt and commercial Pt/C catalysts, and the results were shown in Figure S3. In acid media, the current density and the jf/jb value of 100-SDS-Ti3C2Tx/Pt is obviously higher than that of (46.4 mA cm −2 , 0.94). Furthermore, the CA after 6000 s ( Figure S3b) also  Figure 8a shows the CV curves of the four nanocatalysts in 0.5 mol L −1 H 2 SO 4 +1 mol L −1 C 2 H 5 OH solution. There are two obvious oxidation peaks observed at 0.65 V and 0.46 V, which is assigned to the positive oxidation peak of ethanol and the oxidation peak of the toxic intermediate product during the negative scan. Generally, a higher the peak current of ethanol during forward scanning means a better catalytic performance. The current density of the 100-SDS-Ti 3 C 2 T x /Pt nanocatalyst reaches 50.3 mA cm −2 , which is much higher than 0-SDS-Ti 3 C 2 T x /Pt, 20-SDS-Ti 3 C 2 T x /Pt, and 50-SDS-Ti 3 C 2 T x /Pt, indicating its largest electrocatalytic activity. The ratio (j f /j b ) between the current density of the positive-scan oxidation peak (j f ) and the peak current density (j b ) of the anti-scan oxidation peak (j f /j b ) is employed to study the anti-toxicity of the catalyst during the ethanol oxidation process. The higher ratio (j f /j b ) is, the easier oxidation reaction of ethanol is, and the nanocomposite can adsorb ethanol molecules more efficiently [34,35]. As shown in Figure 8b, it can be clearly found the j f /j b value of 100-SDS-Ti 3 C 2 T x /Pt catalyst is 1.21, which is higher than 50-SDS-Ti 3 C 2 T x /Pt (1.17), 20-SDS-Ti 3 C 2 T x /Pt (0.94), and 0-SDS-Ti 3 C 2 T x /Pt (0.97), further demonstrating its high electrocatalytic activity and anti-poisoning ability for ethanol oxidation in acidic media. Owing to the superior electrocatalytic activity of 100-SDS-Ti 3 C 2 T x /Pt over other catalyst, we also compared the electrochemical performance of 100-SDS-Ti 3 C 2 T x /Pt and commercial Pt/C catalysts, and the results were shown in Figure S3. In acid media, the current density and the j f /j b value of 100-SDS-Ti 3 C 2 T x /Pt is obviously higher than that of (46.4 mA cm −2 , 0.94). Furthermore, the CA after 6000 s ( Figure S3b) also showed that, the current decay of 100-SDS-Ti 3 C 2 T x /Pt is much slower than that of Pt/C catalyst. Taken together, these results indicated that the 100-SDS-Ti 3 C 2 T x /Pt have remarkable catalytic and long-term stability for ethanol oxidation in acid solution. The electrocatalytic activity of 100-SDS-Ti 3 C 2 T x /Pt, 50-SDS-Ti 3 C 2 T x /Pt, 20-SDS-Ti 3 C 2 T x /Pt, and 0-SDS-Ti 3 C 2 T x /Pt catalysts in alkaline media is shown in Figure 8c. Similarly, oxidation peaks appear during the positive scanning process and the reverse scanning process. The oxidation peak during the positive scanning process is the direct oxidation peak of ethanol, and the oxidation peak during the negative scanning process is the re-oxidation of the intermediate product.
In the mixture solution of 1 mol L −1 KOH and 1 mol L −1 C 2 H 5 OH, the direct oxidation peak current densities of ethanol are 61.8, 37.8, 24.6, and 5.5 cm −2 with the electrode of 100-SDS-Ti 3 C 2 T x /Pt, 50-SDS-Ti 3 C 2 T x /Pt, 20-SDS-Ti 3 C 2 T x /Pt, and 0-SDS-Ti 3 C 2 T x /Pt, respectively. Obviously, the 100-SDS-Ti 3 C 2 T x /Pt catalyst obviously has the largest current density, indicating the highest electrocatalytic activity in the alkaline medium. The ratios of j f /j b for 100-SDS-Ti 3 C 2 T x /Pt, 50-SDS-Ti 3 C 2 T x /Pt, 20-SDS-Ti 3 C 2 T x /Pt, and 0-SDS-Ti 3 C 2 T x /Pt are 1.40, 1.58, 2.66 and 1.50, respectively, as shown in Figure 8d. The 100-SDS-Ti 3 C 2 T x /Pt catalyst has a lower j f /j b value, which indicates that the catalyst with the highest catalytic activity could also bring in more intermediate products in the secondary oxidation process. Figure S4 shows the electrocatalytic activity of the 100-SDS-Ti 3 C 2 T x /Pt and commercial Pt/C catalysts for ethanol oxidation in alkaline solution. The forward anodic peak value of 100-SDS-Ti 3 C 2 T x /Pt is slightly higher than 48.0 cm −2 for commercial Pt/C catalyst (Figure 4a). After 6000 s of CA (Figure 4b), the residue current of 100-SDS-Ti 3 C 2 T x /Pt is much higher that of Pt-C, indicating a superior stability and catalytic activity towards ethanol oxidation in alkaline solution. In addition, it is observed that the electrocatalytic activity of the 100-SDS-Ti 3 C 2 T x /Pt nanocatalyst in the alkaline medium is significantly stronger than that of in the acidic medium. This is because ethanol oxidation involves multiple steps in the dehydrogenation process. The platinum on the catalyst surface is easily oxidized by the surrounding water molecules to form the intermediate species, Pt+H 2 O→Pt-OH ads +H + +e − . In the acidic solutions, due to the low content of oxygencontaining substances OH ads , the ability of Pt to catalyze the oxidative dehydrogenation of ethanol is relatively poor [36]. However, the alkaline solution contains abundant OH groups, which makes intermediate products prone to dehydrogenation reaction, significantly improving the electrocatalytic efficiency of ethanol oxidation. The reaction is as follows: CH 3 CH 2 OH+2OH − →CH 3 COOH+2H 2 O+2e − . The process of alkaline oxidation can be deduced that ethanol molecules are first adsorbed on the catalyst and interact with the OH ads in the solution, then gradually dehydrogenate to form CH 3 CO − or CH 3 COO − , and finally the C-C bonds are break to form CO 2 .
ethanol is relatively poor [36]. However, the alkaline solution contains abundant OH groups, which makes intermediate products prone to dehydrogenation reaction, significantly improving the electrocatalytic efficiency of ethanol oxidation. The reaction is as follows: CH3CH2OH+2OH − →CH3COOH+2H2O+2e − . The process of alkaline oxidation can be deduced that ethanol molecules are first adsorbed on the catalyst and interact with the OHads in the solution, then gradually dehydrogenate to form CH3CO − or CH3COO − , and finally the C-C bonds are break to form CO2. In order to compare the stability of the 0-SDS-Ti3C2Tx/Pt, 20-SDS-Ti3C2Tx/Pt, 50-SDS-Ti3C2Tx/Pt and 100-SDS Ti3C2Tx/Pt catalysts in the electrocatalytic process, the chronoamperometry was employed to analyze the performance of catalysts in the mixed solutions of 0.5 mol L −1 H2SO4+1 mol L −1 C2H5OH and 1 mol L −1 KOH+ 1 mol L −1 C2H5OH. Generally, the attenuation of the oxidation current density means the decrease of catalyst activity and the catalyst poisoning, which results from the adsorption of the CO intermediate product In order to compare the stability of the 0-SDS-Ti 3 C 2 T x /Pt, 20-SDS-Ti 3 C 2 T x /Pt, 50-SDS-Ti 3 C 2 T x /Pt and 100-SDS Ti 3 C 2 T x /Pt catalysts in the electrocatalytic process, the chronoamperometry was employed to analyze the performance of catalysts in the mixed solutions of 0.5 mol L −1 H 2 SO 4 +1 mol L −1 C 2 H 5 OH and 1 mol L −1 KOH+ 1 mol L −1 C 2 H 5 OH. Generally, the attenuation of the oxidation current density means the decrease of catalyst activity and the catalyst poisoning, which results from the adsorption of the CO intermediate product from the oxidation of ethanol on the surface of Pt [37,38]. As shown in Figure 9a, the current density of all catalysts decreases significantly in the beginning and then gradually stabilized. The results show that the 100-SDS-Ti 3 C 2 T x /Pt nanocomposite still has the highest current density after 6000 s chronoamperometry test, indicating its better anti-poisoning ability and stability. Besides, in 1 mol L −1 KOH+1 mol L −1 C 2 H 5 OH solution, the final steady-state current density of the 100-SDS-Ti 3 C 2 T x /Pt catalyst is also highest than others (Figure 9b). These results confirm that 100-SDS-Ti 3 C 2 T x /Pt has the best anti-poisoning ability and stability during the electrocatalytic oxidation of ethanol, no matter in the acid or the alkaline media, which is consistent with the previous CV results. Moreover, we measured the repeatability of electrocatalytic activity for the 100-SDS-Ti 3 C 2 T x /Pt catalyst, and the results were shown in Figure S5. After the catalyst has been put aside for one month, the current density of 100-SDS-Ti 3 C 2 T x /Pt still kept 92.8% and 87.2% of its initial current density for acid ( Figure S5a) and alkaline solution ( Figure S5b). Although the higher catalytic activity of alkaline solution that acid solution, the100-SDS-Ti 3 C 2 T x /Pt catalyst displayed a better repeatability in acid solution.
the alkaline media, which is consistent with the previous CV results. Moreover, we measured the repeatability of electrocatalytic activity for the 100-SDS-Ti3C2Tx/Pt catalyst, and the results were shown in Figure S5. After the catalyst has been put aside for one month, the current density of 100-SDS-Ti3C2Tx/Pt still kept 92.8% and 87.2% of its initial current density for acid ( Figure S5a) and alkaline solution ( Figure S5b). Although the higher catalytic activity of alkaline solution that acid solution, the100-SDS-Ti3C2Tx/Pt catalyst displayed a better repeatability in acid solution. The generally accepted oxidation mechanism of SDS-Ti3C2Tx/Pt catalysts is described in the Figure 10 and the following equation from the previous research [39,40]. The electrocatalytic oxidation mechanism of ethanol on Pt electrode involves parallel reaction and continuous reaction mechanism, the main product is CH3COOH or other products such as CH3CHO, CH3, CO2 and CO. Most specifically, ethanol is first adsorbed the surface of Pt and occurs the oxidation to CH3CHOads (Equations (1) and (2)). The produced poisonous intermediates Pt-(CH3CHO)ads occupy most of the active sites to form catalyst deactivation. The Pt-(CH3CHO)ads are oxidized to acetic acid by these active Pt-containing species and adsorbed Pt is meanwhile released, which is the rate-determining step in this process(Equation (3)).

Pt + C2H5OH→Pt-C2H5OHads
(1) Pt-C2H5OHads + 2OH -→Pt-(CH3CHO)ads + 2H2O + 2e − Pt-(CH3CHO)ads + Pt-(OH)ads + OH − →2Pt + CH3COOH + H2O + e − In the ethanol oxidation process, there must be sufficient intermediate adsorption species and OH − group on the catalyst surface. The 100-SDS-Ti3C2Tx/Pt catalyst could provide more active sites over other catalysts, it is beneficial to dissociation and adsorption of ethanol molecular and display a good catalytic performance. The generally accepted oxidation mechanism of SDS-Ti 3 C 2 T x /Pt catalysts is described in the Figure 10 and the following equation from the previous research [39,40]. The electrocatalytic oxidation mechanism of ethanol on Pt electrode involves parallel reaction and continuous reaction mechanism, the main product is CH 3 COOH or other products such as CH 3 CHO, CH 3 , CO 2 and CO. Most specifically, ethanol is first adsorbed the surface of Pt and occurs the oxidation to CH 3 CHO ads (Equations (1) and (2)). The produced poisonous intermediates Pt-(CH 3 CHO) ads occupy most of the active sites to form catalyst deactivation. The Pt-(CH 3 CHO) ads are oxidized to acetic acid by these active Pt-containing species and adsorbed Pt is meanwhile released, which is the rate-determining step in this process(Equation (3)

Conclusions
In this paper, a two-step synthesis method was used to synthesize the SDS-Ti3C2Tx/Pt nanocomposite catalyst. The effect of the SDS content on the dispersion of Pt nanoparticles was studied and the electrocatalytic performance for ethanol oxidation of the SDS-Ti3C2Tx/Pt nanocomposite catalyst in the acidic and in the alkaline media was also investigated. The SDS-Ti3C2Tx supported catalysts not only improve the catalytic performance of Pt catalyst towards EOR, but also considerably decrease the cost of noble catalyst. The electrocatalytic activity of the SDS-Ti3C2Tx/Pt nanocomposite catalyst reaches the maximum when 100 mg SDS is added. The improved electrocatalytic activity and anti-poisoning ability of SDS-Ti3C2Tx/Pt is attributed to the SDS modification for Ti3C2Tx, which increases the dispersion and the active sites of Pt nanoparticles. This work provides important basics for the synthesis and application of Pt nanoparticle in catalysis.
Supplementary Materials: The following are available online at www.mdpi.com/xxx/s1, Figure S1-S5: Raman spectra, FT-IR spectra and CV curves.  In the ethanol oxidation process, there must be sufficient intermediate adsorption species and OH − group on the catalyst surface. The 100-SDS-Ti 3 C 2 T x /Pt catalyst could provide more active sites over other catalysts, it is beneficial to dissociation and adsorption of ethanol molecular and display a good catalytic performance.

Conclusions
In this paper, a two-step synthesis method was used to synthesize the SDS-Ti 3 C 2 T x /Pt nanocomposite catalyst. The effect of the SDS content on the dispersion of Pt nanoparticles was studied and the electrocatalytic performance for ethanol oxidation of the SDS-Ti 3 C 2 T x /Pt nanocomposite catalyst in the acidic and in the alkaline media was also investigated. The SDS-Ti 3 C 2 T x supported catalysts not only improve the catalytic performance of Pt catalyst towards EOR, but also considerably decrease the cost of noble catalyst. The electrocatalytic activity of the SDS-Ti 3 C 2 T x /Pt nanocomposite catalyst reaches the maximum when 100 mg SDS is added. The improved electrocatalytic activity and anti-poisoning ability of SDS-Ti 3 C 2 T x /Pt is attributed to the SDS modification for Ti 3 C 2 T x , which increases the dispersion and the active sites of Pt nanoparticles. This work provides important basics for the synthesis and application of Pt nanoparticle in catalysis.

Data Availability Statement:
The data is available on reasonable request from the corresponding author.